A magnetic core is a piece of magnetic material with a high magnetic permeability used to confine and guide magnetic fields in electrical, electromechanical and magnetic devices such as electromagnets, transformers, electric motors, generators, inductors, magnetic recording heads, and magnetic assemblies. It is made of ferromagnetic metal such as iron, or ferrimagnetic compounds such as ferrites. The high permeability, relative to the surrounding air, causes the magnetic field lines to be concentrated in the core material. The magnetic field is often created by a coil of wire around the core that carries a current. The presence of the core can increase the magnetic field of a coil by a factor of several thousand over what it would be without the core.
The use of a magnetic core can enormously concentrate the strength and increase the effect of magnetic fields produced by electric currents and permanent magnets. The properties of a device will depend crucially on the following factors:
- the geometry of the magnetic core.
- the amount of air gap in the magnetic circuit.
- the properties of the core material (especially permeability and hysteresis).
- the operating temperature of the core.
- whether the core is laminated to reduce eddy currents.
In many applications it is undesirable for the core to retain magnetization when the applied field is removed. This property, called hysteresis can cause energy losses in applications such as transformers. Therefore, 'soft' magnetic materials with low hysteresis, such as silicon steel, rather than the 'hard' magnetic materials used for permanent magnets, are usually used in cores.
- 1 Magnetic core materials
- 2 Commonly used structures
- 3 AL value
- 4 Core loss
- 5 See also
- 6 References
- 7 External links
Magnetic core materials
Having no magnetically active core material (an "air core") provides very low inductance in most situations, so a wide range of high-permeability materials are used to concentrate the field. Most high-permeability material are ferromagnetic or ferrimagnetic.
"Soft" (annealed) iron is used in magnetic assemblies, direct current (DC) electromagnets and in some electric motors; and it can create a concentrated field that is as much as 50,000 times more intense than an air core.
Iron is desirable to make magnetic cores, as it can withstand high levels of magnetic field without saturating (up to 2.16 teslas at ambient temperature.) Annealed iron is used because, unlike "hard" iron, it has low coercivity and so does not remain magnetised when the field is removed, which is often important in applications where the magnetic field is required to be repeatedly switched.
Due to the electrical conductivity of the metal, when a solid one-piece metal core is used in alternating current (AC) applications such as transformers and inductors, the changing magnetic field induces large eddy currents circulating within it, closed loops of electric current in planes perpendicular to the field. The current flowing through the resistance of the metal heats it by Joule heating, causing significant power losses. Therefore solid iron cores are not used in transformers or inductors, they are replaced by laminated or powdered iron cores, or nonconductive cores like ferrite.
Laminated silicon steel
Laminated magnetic cores are made of stacks of thin iron sheets coated with an insulating layer, lying as much as possible parallel with the lines of flux. The layers of insulation serve as a barrier to eddy currents, so eddy currents can only flow in narrow loops within the thickness of each single lamination. Since the current in an an eddy current loop is proportional to the area of the loop, this prevents most of the current from flowing, reducing eddy currents to a very small level. Since power dissipated is proportional to the square of the current, breaking a large core into narrow laminations reduces the power losses drastically. From this, it can be seen that the thinner the laminations, the lower the eddy current losses.
A small addition of silicon to iron (around 3%) results in a dramatic increase of the resistivity of the metal, up to four times higher. The higher resistivity reduces the eddy currents, so silicon steel is used in transformer cores. Further increase in silicon concentration impairs the steel's mechanical properties, causing difficulties for rolling due to brittleness.
Among the two types of silicon steel, grain-oriented (GO) and grain non-oriented (GNO), GO is most desirable for magnetic cores. It is anisotropic, offering better magnetic properties than GNO in one direction. As the magnetic field in inductor and transformer cores is always along the same direction, it is an advantage to use grain oriented steel in the preferred orientation. Rotating machines, where the direction of the magnetic field can change, gain no benefit from grain-oriented steel.
A family of specialized alloys exists for magnetic core applications. Examples are mu-metal, permalloy, and supermalloy. They can be manufactured as stampings or as long ribbons for tape wound cores. Some alloys, e.g. Sendust, are manufactured as powder and sintered to shape.
Many materials require careful heat treatment to reach their magnetic properties, and lose them when subjected to mechanical or thermal abuse. For example, the permeability of mu-metal increases about 40 times after annealing in hydrogen atmosphere in a magnetic field; subsequent sharper bends disrupt its grain alignment, leading to localized loss of permeability; this can be regained by repeating the annealing step.
Amorphous metal is a variety of alloys (e.g. Metglas) that are non-crystalline or glassy. These are being used to create high-efficiency transformers. The materials can be highly responsive to magnetic fields for low hysteresis losses, and they can also have lower conductivity to reduce eddy current losses. China is currently making widespread industrial and power grid usage of these transformers for new installations.
Powdered cores made of carbonyl iron, a highly pure iron, have high stability of parameters across a wide range of temperatures and magnetic flux levels, with excellent Q factors between 50 kHz and 200 MHz. Carbonyl iron powders are basically constituted of micrometer-size spheres of iron coated in a thin layer of electrical insulation. This is equivalent to a microscopic laminated magnetic circuit (see silicon steel, above), hence reducing the eddy currents, particularly at very high frequencies.
Powdered cores made of hydrogen reduced iron have higher permeability but lower Q. They are used mostly for electromagnetic interference filters and low-frequency chokes, mainly in switched-mode power supplies.
Ferrite ceramics are used for high-frequency applications. The ferrite materials can be engineered with a wide range of parameters. As ceramics, they are essentially insulators, which prevents eddy currents, although losses such as hysteresis losses can still occur.
A coil not containing a magnetic core is called an air core. This includes coils wound on a plastic or ceramic form in addition to those made of stiff wire that are self-supporting and have air inside them. Air core coils generally have a much lower inductance than similarly sized ferromagnetic core coils, but are used in radio frequency circuits to prevent energy losses called core losses that occur in magnetic cores. The absence of normal core losses permits a higher Q factor, so air core coils are used in high frequency resonant circuits, such as up to a few megahertz. However, losses such as proximity effect and dielectric losses are still present. Air cores are also used when field strengths above around 2 Tesla are required as they are not subject to saturation.
Commonly used structures
Straight cylindrical rod
Most commonly made of ferrite or powdered iron, and used in radios especially for tuning an inductor. The coil is wound around the rod, or a coil form with the rod inside. Moving the rod in or out of the coil changes the flux through the coil, and can be used to adjust the inductance. Often the rod is threaded to allow adjustment with a screwdriver. In radio circuits, a blob of wax or resin is used once the inductor has been tuned to prevent the core from moving.
The presence of the high permeability core increases the inductance, but the magnetic field lines must still pass through the air from one end of the rod to the other. The air path ensures that the inductor remains linear. In this type of inductor radiation occurs at the end of the rod and electromagnetic interference may be a problem in some circumstances.
Single "I" core
Like a cylindrical rod but square, rarely used on its own. This type of core is most likely to be found in car ignition coils.
"C" or "U" core
U and C-shaped cores are used with I or another C or U core to make a square closed core, the simplest closed core shape. Windings may be put on one or both legs of the core.
E-shaped core are more symmetric solutions to form a closed magnetic system. Most of the time, the electric circuit is wound around the center leg, whose section area is twice that of each individual outer leg. In 3-phase transformer cores, the legs are of equal size, and all three legs are wound.
"E" and "I" core
Sheets of suitable iron stamped out in shapes like the (sans-serif) letters "E" and "I", are stacked with the "I" against the open end of the "E" to form a 3-legged structure. Coils can be wound around any leg, but usually the center leg is used. This type of core is frequently used for power transformers, autotransformers, and inductors.
Pair of "E" cores
Again used for iron cores. Similar to using an "E" and "I" together, a pair of "E" cores will accommodate a larger coil former and can produce a larger inductor or transformer. If an air gap is required, the centre leg of the "E" is shortened so that the air gap sits in the middle of the coil to minimize fringing and reduce electromagnetic interference.
Usually ferrite or similar. This is used for inductors and transformers. The shape of a pot core is round with an internal hollow that almost completely encloses the coil. Usually a pot core is made in two halves which fit together around a coil former (bobbin). This design of core has a shielding effect, preventing radiation and reducing electromagnetic interference.
Main article: Toroidal inductors and transformers
This design is based on a toroid (the same shape as a doughnut). The coil is wound through the hole in the torus and around the outside. An ideal coil is distributed evenly all around the circumference of the torus. The symmetry of this geometry creates a magnetic field of circular loops inside the core, and the lack of sharp bends will constrain virtually all of the field to the core material. This not only makes a highly efficient transformer, but also reduces the electromagnetic interference radiated by the coil.
It is popular for applications where the desirable features are: high specific power per mass and volume, low mains hum, and minimal electromagnetic interference. One such application is the power supply for a hi-fi audio amplifier. The main drawback that limits their use for general purpose applications is the inherent difficulty of winding wire through the center of a torus.
Unlike a split core (a core made of two elements, like a pair of E cores), specialized machinery is required for automated winding of a toroidal core. Toroids have less audible noise, such as mains hum, because the magnetic forces do not exert bending moment on the core. The core is only in compression or tension, and the circular shape is more stable mechanically.
Ring or bead
The ring is essentially identical in shape and performance to the toroid, except that inductors commonly pass only through the center of the core, without wrapping around the core multiple times.
The ring core may also be composed of two separate C-shaped hemispheres secured together within a plastic shell, permitting it to be placed on finished cables with large connectors already installed, that would prevent threading the cable through the small inner diameter of a solid ring.
A planar core consists of two flat pieces of magnetic material, one above and one below the coil. It is typically used with a flat coil that is part of a printed circuit board. This design is excellent for mass production and allows a high power, small volume transformer to be constructed for low cost. It is not as ideal as either a pot core or toroidal core but costs less to produce.
The AL value of a core configuration is frequently specified by manufacturers. The relationship between inductance and AL number in the linear portion of the magnetisation curve is defined to be:
where n is the number of turns, L is the inductance (e.g. in nH) and AL is expressed in inductance per turn squared (e.g. in nH/n2).
|This section does not cite any sources. (January 2016) (Learn how and when to remove this template message)|
When the core is subjected to a changing magnetic field, as it is in devices that use AC current such as transformers, inductors, and AC motors and alternators, some of the power that would ideally be transferred through the device is lost in the core, dissipated as heat and sometimes noise. The losses are often described as being in three categories:
- Hysteresis losses - When the magnetic field through the core changes, the magnetization of the core material changes by expansion and contraction of the tiny magnetic domains it is composed of, due to movement of the domain walls. This process causes losses, because the domain walls get "snagged" on defects in the crystal structure and then "snap" past them, dissipating energy as heat. This is called hysteresis loss. It can be seen in the graph of the B field versus the H field for the material, which has the form of a closed loop. The amount of energy lost in the material in one cycle of the applied field is proportional to the area inside the hysteresis loop. Since the energy lost in each cycle is constant, hysteresis power losses increase proportionally with frequency.
- Eddy-current losses - If the core is electrically conductive, the changing magnetic field induces circulating loops of current in it, called eddy currents, due to electromagnetic induction. The loops flow perpendicular to the magnetic field axis. The energy of the currents is dissipated as heat in the resistance of the core material. The power loss is proportional to the area of the loops and inversely proportional to the resistivity of the core material. Eddy current losses can be reduced by making the core out of thin laminations which have an insulating coating, or alternatively, making the core of a magnetic material with high electrical resistance, like ferrite.
- Anomalous losses - By definition, this category includes any losses in addition to eddy-current and hysteresis losses. This can also be described as broadening of the hysteresis loop with frequency. Physical mechanisms for anomalous loss include localized eddy-current effects near moving domain walls.
- Pole piece
- Choke (electronics)
- Electromagnetic interference
- Ferrite (iron)
- Ferrite (magnet)
- Magnetic core memory
- Toroidal inductors and transformers
- Unintentional radiator
-  - Online calculator for ferrite coil winding calculations.
- What are the bumps at the end of computer cables?
- How to use ferrites for EMI suppression via Wayback Machine by Murata Manufacturing